as aerogel. Variations in synthesis can alter the surface area and pore size of the aerogel. The smaller the pore size the more susceptible the aerogel is to fracture. Waterproofing Aerogel contains particles that are 2–5 nm in diameter. After the process of creating aerogel, it will contain a large amount of hydroxyl groups on the surface. The hydroxyl groups can cause a strong reaction when the aerogel is placed in water, causing it to catastrophically dissolve in the water. One way to waterproof the hydrophilic aerogel is by soaking the aerogel with some chemical base that will replace the surface hydroxyl groups (–OH) with non-polar groups (–OR), a process which is most effective when R is an aliphatic group. Porosity of aerogel There are several ways to determine the porosity of aerogel: the three main methods are gas adsorption, mercury porosimetry, and scattering method. In gas adsorption, nitrogen at its boiling point is adsorbed into the aerogel sample. The gas being adsorbed is dependent on the size of the pores within the sample and on the partial pressure of the gas relative to its saturation pressure. The volume of the gas adsorbed is measured by using the Brunauer, Emmit and Teller formula (BET), which gives the specific surface area of the sample. At high partial pressure in the adsorption/desorption the Kelvin equation gives the pore size distribution of the sample. In mercury porosimetry, the mercury is forced into the aerogel porous system to determine the pores' size, but this method is highly inefficient since the solid frame of aerogel will collapse from the high compressive force. The scattering method involves the angle-dependent deflection of radiation within the aerogel sample. The sample can be solid particles or pores. The radiation goes into the material and determines the fractal geometry of the aerogel pore network. The best radiation wavelengths to use are X-rays and neutrons. Aerogel is also an open porous network: the difference between an open porous network and a closed porous network is that in the open network, gases can enter and leave the substance without any limitation, while a closed porous network traps the gases within the material forcing them to stay within the pores. The high porosity and surface area of silica aerogels allow them to be used in a variety of environmental filtration applications. Materials Silica aerogel Silica aerogels are the most common type of aerogel,